#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/07/4330774.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4330774
loop_
_publ_author_name
'Wei-Qiu Kan'
'Jin Yang'
'Ying-Ying Liu'
'Jian-Fang Ma'
_publ_contact_author_address
;
Department of Chemistry
Northeast Normal University
Changchun 130024
P.R.China
;
_publ_contact_author_email       jianfangma@yahoo.com.cn
_publ_contact_author_fax         +86-431-85098620
_publ_contact_author_name        'Jian-Fang Ma'
_publ_contact_author_phone       +86-431-85098620
_publ_section_title
;
 Series of Inorganic-Organic Hybrid Materials Constructed From
 Octamolybdates and Metal-Organic Frameworks: Syntheses, Structures, and
 Physical Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11266
_journal_page_last               11278
_journal_paper_doi               10.1021/ic300134z
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         'C15 H13 Ag Mo4 N8 O13'
_chemical_formula_sum            'C15 H13 Ag Mo4 N8 O13'
_chemical_formula_weight         1004.96
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                98.289(5)
_cell_angle_beta                 94.162(5)
_cell_angle_gamma                107.191(5)
_cell_formula_units_Z            2
_cell_length_a                   10.385(5)
_cell_length_b                   10.488(5)
_cell_length_c                   12.150(5)
_cell_measurement_reflns_used    3905
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.1708
_cell_measurement_theta_min      2.8926
_cell_volume                     1241.7(10)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0232
_diffrn_reflns_av_sigmaI/netI    0.0434
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            7765
_diffrn_reflns_theta_full        25.35
_diffrn_reflns_theta_max         25.35
_diffrn_reflns_theta_min         2.90
_exptl_absorpt_coefficient_mu    2.822
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.75793
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlis (Oxford Diffraction, 2006)
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.688
_exptl_crystal_description       block
_exptl_crystal_F_000             956
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.20
_refine_diff_density_max         0.487
_refine_diff_density_min         -0.746
_refine_diff_density_rms         0.125
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     370
_refine_ls_number_reflns         4531
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.0386
_refine_ls_R_factor_gt           0.0284
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0238P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0579
_refine_ls_wR_factor_ref         0.0625
_reflns_number_gt                3786
_reflns_number_total             4531
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ic300134z_si_002_6.cif
_cod_data_source_block           compound-6
_cod_original_sg_symbol_Hall     '-p 1'
_cod_database_code               4330774
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ag1 Ag -0.64863(4) -0.44125(4) 0.47735(3) 0.03237(11) Uani 1 1 d .
Mo1 Mo 0.14653(4) 0.43668(4) 0.89023(3) 0.02091(11) Uani 1 1 d .
Mo2 Mo 0.31741(4) 0.58881(4) 1.13435(3) 0.01862(10) Uani 1 1 d .
Mo3 Mo 0.57386(4) 0.47034(4) 1.22357(3) 0.01898(10) Uani 1 1 d .
Mo4 Mo 0.40915(4) 0.32405(4) 0.98325(3) 0.01759(10) Uani 1 1 d .
C1 C -0.4430(5) -0.1733(5) 0.4308(4) 0.0297(11) Uani 1 1 d .
H1 H -0.4619 -0.2154 0.3561 0.036 Uiso 1 1 calc R
C2 C -0.4455(5) -0.1429(5) 0.6046(4) 0.0315(12) Uani 1 1 d .
H2 H -0.4623 -0.1539 0.6773 0.038 Uiso 1 1 calc R
C3 C -0.2736(4) 0.0903(5) 0.6463(4) 0.0279(11) Uani 1 1 d .
H3A H -0.2745 0.1683 0.6123 0.033 Uiso 1 1 calc R
H3B H -0.3048 0.1018 0.7193 0.033 Uiso 1 1 calc R
C4 C -0.0244(4) 0.1361(5) 0.6104(3) 0.0232(10) Uani 1 1 d .
C5 C -0.0088(4) 0.2277(5) 0.5274(3) 0.0224(10) Uani 1 1 d .
C6 C -0.1121(4) 0.2340(5) 0.4503(4) 0.0265(11) Uani 1 1 d .
H6 H -0.2005 0.1776 0.4478 0.032 Uiso 1 1 calc R
C7 C -0.0808(5) 0.3255(5) 0.3778(4) 0.0292(11) Uani 1 1 d .
H7 H -0.1480 0.3316 0.3258 0.035 Uiso 1 1 calc R
C8 C 0.0498(5) 0.4069(5) 0.3831(4) 0.0287(11) Uani 1 1 d .
H8 H 0.0693 0.4686 0.3342 0.034 Uiso 1 1 calc R
C9 C 0.1217(4) 0.3139(5) 0.5256(3) 0.0231(10) Uani 1 1 d .
H9 H 0.1915 0.3096 0.5759 0.028 Uiso 1 1 calc R
C10 C 0.0220(5) 0.0248(5) 0.7304(4) 0.0271(11) Uani 1 1 d .
C11 C 0.0995(5) -0.0313(5) 0.8035(4) 0.0301(11) Uani 1 1 d .
C12 C 0.2354(5) -0.0148(5) 0.7939(4) 0.0344(12) Uani 1 1 d .
H12 H 0.2772 0.0313 0.7397 0.041 Uiso 1 1 calc R
C13 C 0.3074(6) -0.0661(5) 0.8637(4) 0.0409(14) Uani 1 1 d .
H13 H 0.3985 -0.0554 0.8572 0.049 Uiso 1 1 calc R
C14 C 0.1193(7) -0.1498(6) 0.9538(5) 0.0528(16) Uani 1 1 d .
H14 H 0.0814 -0.1955 1.0096 0.063 Uiso 1 1 calc R
C15 C 0.0406(6) -0.1015(5) 0.8841(4) 0.0412(13) Uani 1 1 d .
H15 H -0.0510 -0.1161 0.8914 0.049 Uiso 1 1 calc R
N1 N -0.4991(4) -0.2352(4) 0.5142(3) 0.0302(9) Uani 1 1 d .
N2 N -0.3602(4) -0.0502(4) 0.4632(3) 0.0299(10) Uani 1 1 d .
N3 N -0.3645(3) -0.0324(4) 0.5763(3) 0.0250(9) Uani 1 1 d .
N4 N -0.1371(4) 0.0826(4) 0.6593(3) 0.0251(9) Uani 1 1 d .
N5 N -0.1080(4) 0.0102(4) 0.7365(3) 0.0307(10) Uani 1 1 d .
N6 N 0.0767(4) 0.1007(4) 0.6532(3) 0.0254(9) Uani 1 1 d .
N7 N 0.1515(4) 0.4023(4) 0.4556(3) 0.0247(9) Uani 1 1 d .
N8 N 0.2481(6) -0.1310(5) 0.9410(4) 0.0497(13) Uani 1 1 d .
H8A H 0.2955 -0.1623 0.9847 0.060 Uiso 1 1 calc R
O1 O -0.0064(3) 0.3182(3) 0.8468(3) 0.0326(8) Uani 1 1 d .
O2 O 0.2481(3) 0.4138(3) 0.7664(2) 0.0231(7) Uani 1 1 d .
O3 O 0.1238(3) 0.5842(3) 0.8681(2) 0.0311(8) Uani 1 1 d .
O4 O 0.1606(3) 0.4656(3) 1.0521(2) 0.0257(7) Uani 1 1 d .
O5 O 0.3073(3) 0.7420(3) 1.1095(2) 0.0267(7) Uani 1 1 d .
O6 O 0.2861(3) 0.5895(3) 1.2700(2) 0.0286(8) Uani 1 1 d .
O7 O 0.5215(3) 0.6518(3) 1.1597(2) 0.0198(7) Uani 1 1 d .
O8 O 0.5325(3) 0.5209(3) 1.3535(2) 0.0283(8) Uani 1 1 d .
O9 O 0.5993(3) 0.3189(3) 1.2313(2) 0.0276(7) Uani 1 1 d .
O10 O 0.3907(3) 0.4016(3) 1.1360(2) 0.0194(7) Uani 1 1 d .
O11 O 0.6095(3) 0.4635(3) 1.0382(2) 0.0183(7) Uani 1 1 d .
O12 O 0.4458(3) 0.1831(3) 1.0066(2) 0.0291(8) Uani 1 1 d .
O13 O 0.2372(3) 0.2716(3) 0.9331(2) 0.0258(7) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N7 Ag1 N1 157.82(14) 1_445 .
N7 Ag1 O8 118.95(12) 1_445 1_444
N1 Ag1 O8 80.18(12) . 1_444
O3 Mo1 O1 104.94(16) . .
O3 Mo1 O2 96.95(14) . .
O1 Mo1 O2 102.93(13) . .
O3 Mo1 O4 99.36(14) . .
O1 Mo1 O4 104.88(14) . .
O2 Mo1 O4 142.69(12) . .
O3 Mo1 O13 164.58(13) . .
O1 Mo1 O13 90.41(14) . .
O2 Mo1 O13 77.81(12) . .
O4 Mo1 O13 77.62(11) . .
O3 Mo1 O11 95.33(13) . 2_667
O1 Mo1 O11 159.67(13) . 2_667
O2 Mo1 O11 72.49(10) . 2_667
O4 Mo1 O11 72.76(10) . 2_667
O13 Mo1 O11 69.29(10) . 2_667
O6 Mo2 O5 103.39(14) . .
O6 Mo2 O4 104.01(14) . .
O5 Mo2 O4 103.43(14) . .
O6 Mo2 O7 98.74(13) . .
O5 Mo2 O7 93.89(14) . .
O4 Mo2 O7 147.10(11) . .
O6 Mo2 O10 90.60(12) . .
O5 Mo2 O10 161.36(12) . .
O4 Mo2 O10 84.64(12) . .
O7 Mo2 O10 71.56(11) . .
O6 Mo2 O11 161.97(13) . 2_667
O5 Mo2 O11 93.52(12) . 2_667
O4 Mo2 O11 77.60(11) . 2_667
O7 Mo2 O11 73.57(10) . 2_667
O10 Mo2 O11 71.57(10) . 2_667
O9 Mo3 O8 104.34(15) . .
O9 Mo3 O2 101.98(14) . 2_667
O8 Mo3 O2 100.51(14) . 2_667
O9 Mo3 O10 98.42(14) . .
O8 Mo3 O10 100.27(13) . .
O2 Mo3 O10 146.11(13) 2_667 .
O9 Mo3 O11 94.32(12) . .
O8 Mo3 O11 161.18(13) . .
O2 Mo3 O11 77.62(11) 2_667 .
O10 Mo3 O11 74.10(10) . .
O9 Mo3 O7 163.88(12) . .
O8 Mo3 O7 89.89(13) . .
O2 Mo3 O7 82.42(12) 2_667 .
O10 Mo3 O7 71.16(11) . .
O11 Mo3 O7 71.29(9) . .
O9 Mo3 Mo4 85.26(10) . .
O8 Mo3 Mo4 135.79(11) . .
O2 Mo3 Mo4 119.88(8) 2_667 .
O10 Mo3 Mo4 35.64(7) . .
O11 Mo3 Mo4 42.26(7) . .
O7 Mo3 Mo4 79.18(7) . .
O12 Mo4 O13 106.03(15) . .
O12 Mo4 O7 101.46(13) . 2_667
O13 Mo4 O7 97.18(13) . 2_667
O12 Mo4 O10 100.60(13) . .
O13 Mo4 O10 96.52(12) . .
O7 Mo4 O10 149.61(12) 2_667 .
O12 Mo4 O11 96.56(14) . .
O13 Mo4 O11 157.39(13) . .
O7 Mo4 O11 78.87(11) 2_667 .
O10 Mo4 O11 78.08(10) . .
O12 Mo4 O11 171.78(13) . 2_667
O13 Mo4 O11 82.17(12) . 2_667
O7 Mo4 O11 77.68(11) 2_667 2_667
O10 Mo4 O11 77.49(11) . 2_667
O11 Mo4 O11 75.24(11) . 2_667
O12 Mo4 Mo3 87.56(10) . .
O13 Mo4 Mo3 132.62(9) . .
O7 Mo4 Mo3 124.87(8) 2_667 .
O10 Mo4 Mo3 36.13(8) . .
O11 Mo4 Mo3 46.01(7) . .
O11 Mo4 Mo3 86.33(7) 2_667 .
N2 C1 N1 115.1(4) . .
N2 C1 H1 122.4 . .
N1 C1 H1 122.4 . .
N1 C2 N3 109.9(4) . .
N1 C2 H2 125.1 . .
N3 C2 H2 125.1 . .
N4 C3 N3 110.5(3) . .
N4 C3 H3A 109.6 . .
N3 C3 H3A 109.6 . .
N4 C3 H3B 109.6 . .
N3 C3 H3B 109.6 . .
H3A C3 H3B 108.1 . .
N6 C4 N4 109.5(4) . .
N6 C4 C5 122.7(4) . .
N4 C4 C5 127.7(4) . .
C9 C5 C6 117.6(4) . .
C9 C5 C4 116.5(4) . .
C6 C5 C4 125.9(4) . .
C7 C6 C5 118.9(4) . .
C7 C6 H6 120.6 . .
C5 C6 H6 120.6 . .
C8 C7 C6 119.3(4) . .
C8 C7 H7 120.4 . .
C6 C7 H7 120.4 . .
N7 C8 C7 123.2(5) . .
N7 C8 H8 118.4 . .
C7 C8 H8 118.4 . .
N7 C9 C5 123.4(4) . .
N7 C9 H9 118.3 . .
C5 C9 H9 118.3 . .
N5 C10 N6 114.1(4) . .
N5 C10 C11 122.1(5) . .
N6 C10 C11 123.7(4) . .
C15 C11 C12 118.4(5) . .
C15 C11 C10 121.2(5) . .
C12 C11 C10 120.4(5) . .
C13 C12 C11 119.9(5) . .
C13 C12 H12 120.0 . .
C11 C12 H12 120.0 . .
N8 C13 C12 120.0(6) . .
N8 C13 H13 120.0 . .
C12 C13 H13 120.0 . .
N8 C14 C15 119.9(6) . .
N8 C14 H14 120.1 . .
C15 C14 H14 120.1 . .
C11 C15 C14 119.2(6) . .
C11 C15 H15 120.4 . .
C14 C15 H15 120.4 . .
C2 N1 C1 102.9(4) . .
C2 N1 Ag1 135.9(3) . .
C1 N1 Ag1 121.1(3) . .
C1 N2 N3 101.7(4) . .
C2 N3 N2 110.4(4) . .
C2 N3 C3 130.2(4) . .
N2 N3 C3 118.9(4) . .
C4 N4 N5 109.8(4) . .
C4 N4 C3 133.2(4) . .
N5 N4 C3 117.0(4) . .
C10 N5 N4 102.6(4) . .
C4 N6 C10 104.0(4) . .
C9 N7 C8 117.6(4) . .
C9 N7 Ag1 121.0(3) . 1_665
C8 N7 Ag1 120.6(3) . 1_665
C14 N8 C13 122.6(5) . .
C14 N8 H8A 118.7 . .
C13 N8 H8A 118.7 . .
Mo3 O2 Mo1 117.91(14) 2_667 .
Mo2 O4 Mo1 118.86(15) . .
Mo4 O7 Mo2 108.80(13) 2_667 .
Mo4 O7 Mo3 109.83(11) 2_667 .
Mo2 O7 Mo3 103.47(13) . .
Mo3 O8 Ag1 149.04(16) . 1_666
Mo4 O10 Mo3 108.23(12) . .
Mo4 O10 Mo2 110.40(13) . .
Mo3 O10 Mo2 105.62(12) . .
Mo4 O11 Mo3 91.74(10) . .
Mo4 O11 Mo2 91.83(9) . 2_667
Mo3 O11 Mo2 162.00(14) . 2_667
Mo4 O11 Mo4 104.76(11) . 2_667
Mo3 O11 Mo4 98.58(9) . 2_667
Mo2 O11 Mo4 97.56(11) 2_667 2_667
Mo4 O11 Mo1 163.51(14) . 2_667
Mo3 O11 Mo1 85.82(9) . 2_667
Mo2 O11 Mo1 85.78(9) 2_667 2_667
Mo4 O11 Mo1 91.73(10) 2_667 2_667
Mo4 O13 Mo1 116.81(16) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ag1 N7 2.203(4) 1_445
Ag1 N1 2.218(4) .
Ag1 O8 2.577(3) 1_444
Mo1 O3 1.688(3) .
Mo1 O1 1.693(3) .
Mo1 O2 1.926(3) .
Mo1 O4 1.935(3) .
Mo1 O13 2.305(3) .
Mo1 O11 2.474(3) 2_667
Mo2 O6 1.702(3) .
Mo2 O5 1.708(3) .
Mo2 O4 1.863(3) .
Mo2 O7 2.011(3) .
Mo2 O10 2.308(3) .
Mo2 O11 2.328(3) 2_667
Mo3 O9 1.699(3) .
Mo3 O8 1.717(3) .
Mo3 O2 1.873(3) 2_667
Mo3 O10 1.986(3) .
Mo3 O11 2.303(3) .
Mo3 O7 2.344(3) .
Mo3 Mo4 3.1996(11) .
Mo4 O12 1.688(3) .
Mo4 O13 1.740(3) .
Mo4 O7 1.950(3) 2_667
Mo4 O10 1.963(3) .
Mo4 O11 2.153(3) .
Mo4 O11 2.342(3) 2_667
C1 N2 1.308(6) .
C1 N1 1.356(6) .
C1 H1 0.9300 .
C2 N1 1.319(6) .
C2 N3 1.323(6) .
C2 H2 0.9300 .
C3 N4 1.442(6) .
C3 N3 1.456(5) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 N6 1.310(6) .
C4 N4 1.359(5) .
C4 C5 1.475(6) .
C5 C9 1.392(6) .
C5 C6 1.396(6) .
C6 C7 1.379(7) .
C6 H6 0.9300 .
C7 C8 1.363(6) .
C7 H7 0.9300 .
C8 N7 1.342(6) .
C8 H8 0.9300 .
C9 N7 1.332(6) .
C9 H9 0.9300 .
C10 N5 1.322(6) .
C10 N6 1.366(6) .
C10 C11 1.451(7) .
C11 C15 1.380(7) .
C11 C12 1.386(7) .
C12 C13 1.359(7) .
C12 H12 0.9300 .
C13 N8 1.321(7) .
C13 H13 0.9300 .
C14 N8 1.317(8) .
C14 C15 1.382(8) .
C14 H14 0.9300 .
C15 H15 0.9300 .
N2 N3 1.367(5) .
N4 N5 1.360(5) .
N7 Ag1 2.203(4) 1_665
N8 H8A 0.8600 .
O2 Mo3 1.873(3) 2_667
O7 Mo4 1.950(3) 2_667
O8 Ag1 2.577(3) 1_666
O11 Mo2 2.328(3) 2_667
O11 Mo4 2.342(3) 2_667
O11 Mo1 2.474(3) 2_667
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N8 H8A O5 0.86 1.95 2.726(6) 149.3 1_545
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O9 Mo3 Mo4 O12 -0.20(14) . .
O8 Mo3 Mo4 O12 -105.93(19) . .
O2 Mo3 Mo4 O12 100.91(15) 2_667 .
O10 Mo3 Mo4 O12 -111.77(18) . .
O11 Mo3 Mo4 O12 101.54(15) . .
O7 Mo3 Mo4 O12 175.56(13) . .
O9 Mo3 Mo4 O13 109.46(18) . .
O8 Mo3 Mo4 O13 3.7(2) . .
O2 Mo3 Mo4 O13 -149.43(18) 2_667 .
O10 Mo3 Mo4 O13 -2.1(2) . .
O11 Mo3 Mo4 O13 -148.80(19) . .
O7 Mo3 Mo4 O13 -74.78(16) . .
O9 Mo3 Mo4 O7 -102.48(14) . 2_667
O8 Mo3 Mo4 O7 151.78(19) . 2_667
O2 Mo3 Mo4 O7 -1.37(15) 2_667 2_667
O10 Mo3 Mo4 O7 145.95(18) . 2_667
O11 Mo3 Mo4 O7 -0.74(14) . 2_667
O7 Mo3 Mo4 O7 73.28(13) . 2_667
O9 Mo3 Mo4 O10 111.57(18) . .
O8 Mo3 Mo4 O10 5.8(2) . .
O2 Mo3 Mo4 O10 -147.32(19) 2_667 .
O11 Mo3 Mo4 O10 -146.69(19) . .
O7 Mo3 Mo4 O10 -72.67(16) . .
O9 Mo3 Mo4 O11 -101.74(15) . .
O8 Mo3 Mo4 O11 152.52(19) . .
O2 Mo3 Mo4 O11 -0.63(14) 2_667 .
O10 Mo3 Mo4 O11 146.69(18) . .
O7 Mo3 Mo4 O11 74.02(12) . .
O9 Mo3 Mo4 O11 -174.70(12) . 2_667
O8 Mo3 Mo4 O11 79.56(17) . 2_667
O2 Mo3 Mo4 O11 -73.60(13) 2_667 2_667
O10 Mo3 Mo4 O11 73.73(16) . 2_667
O11 Mo3 Mo4 O11 -72.96(13) . 2_667
O7 Mo3 Mo4 O11 1.05(9) . 2_667
N6 C4 C5 C9 -22.9(6) . .
N4 C4 C5 C9 152.8(4) . .
N6 C4 C5 C6 156.2(4) . .
N4 C4 C5 C6 -28.1(7) . .
C9 C5 C6 C7 -0.8(6) . .
C4 C5 C6 C7 -179.9(4) . .
C5 C6 C7 C8 0.1(6) . .
C6 C7 C8 N7 0.5(7) . .
C6 C5 C9 N7 0.9(6) . .
C4 C5 C9 N7 -179.9(4) . .
N5 C10 C11 C15 -0.8(7) . .
N6 C10 C11 C15 176.6(4) . .
N5 C10 C11 C12 179.5(4) . .
N6 C10 C11 C12 -3.1(7) . .
C15 C11 C12 C13 -0.7(7) . .
C10 C11 C12 C13 179.1(4) . .
C11 C12 C13 N8 -0.3(7) . .
C12 C11 C15 C14 1.5(7) . .
C10 C11 C15 C14 -178.2(4) . .
N8 C14 C15 C11 -1.5(8) . .
N3 C2 N1 C1 1.0(5) . .
N3 C2 N1 Ag1 -176.6(3) . .
N2 C1 N1 C2 -0.5(6) . .
N2 C1 N1 Ag1 177.5(3) . .
N7 Ag1 N1 C2 72.0(6) 1_445 .
O8 Ag1 N1 C2 -136.7(5) 1_444 .
N7 Ag1 N1 C1 -105.2(4) 1_445 .
O8 Ag1 N1 C1 46.0(4) 1_444 .
N1 C1 N2 N3 -0.2(5) . .
N1 C2 N3 N2 -1.2(6) . .
N1 C2 N3 C3 -173.3(4) . .
C1 N2 N3 C2 0.8(5) . .
C1 N2 N3 C3 173.9(4) . .
N4 C3 N3 C2 96.0(6) . .
N4 C3 N3 N2 -75.5(5) . .
N6 C4 N4 N5 0.1(5) . .
C5 C4 N4 N5 -176.1(4) . .
N6 C4 N4 C3 178.8(4) . .
C5 C4 N4 C3 2.7(8) . .
N3 C3 N4 C4 100.9(6) . .
N3 C3 N4 N5 -80.4(5) . .
N6 C10 N5 N4 -0.7(5) . .
C11 C10 N5 N4 176.9(4) . .
C4 N4 N5 C10 0.3(4) . .
C3 N4 N5 C10 -178.6(4) . .
N4 C4 N6 C10 -0.5(5) . .
C5 C4 N6 C10 175.9(4) . .
N5 C10 N6 C4 0.7(5) . .
C11 C10 N6 C4 -176.8(4) . .
C5 C9 N7 C8 -0.3(6) . .
C5 C9 N7 Ag1 169.2(3) . 1_665
C7 C8 N7 C9 -0.4(6) . .
C7 C8 N7 Ag1 -170.0(3) . 1_665
C15 C14 N8 C13 0.5(8) . .
C12 C13 N8 C14 0.4(8) . .
O3 Mo1 O2 Mo3 71.35(19) . 2_667
O1 Mo1 O2 Mo3 178.48(18) . 2_667
O4 Mo1 O2 Mo3 -44.1(3) . 2_667
O13 Mo1 O2 Mo3 -93.93(18) . 2_667
O11 Mo1 O2 Mo3 -22.06(15) 2_667 2_667
O6 Mo2 O4 Mo1 177.46(16) . .
O5 Mo2 O4 Mo1 69.70(18) . .
O7 Mo2 O4 Mo1 -50.1(3) . .
O10 Mo2 O4 Mo1 -93.26(17) . .
O11 Mo2 O4 Mo1 -20.99(15) 2_667 .
O3 Mo1 O4 Mo2 -72.55(19) . .
O1 Mo1 O4 Mo2 179.14(17) . .
O2 Mo1 O4 Mo2 42.2(3) . .
O13 Mo1 O4 Mo2 92.05(17) . .
O11 Mo1 O4 Mo2 20.16(15) 2_667 .
O6 Mo2 O7 Mo4 -175.47(15) . 2_667
O5 Mo2 O7 Mo4 -71.27(15) . 2_667
O4 Mo2 O7 Mo4 51.0(3) . 2_667
O10 Mo2 O7 Mo4 96.82(13) . 2_667
O11 Mo2 O7 Mo4 21.25(12) 2_667 2_667
O6 Mo2 O7 Mo3 67.78(14) . .
O5 Mo2 O7 Mo3 171.98(12) . .
O4 Mo2 O7 Mo3 -65.7(3) . .
O10 Mo2 O7 Mo3 -19.92(9) . .
O11 Mo2 O7 Mo3 -95.49(11) 2_667 .
O9 Mo3 O7 Mo4 -41.2(5) . 2_667
O8 Mo3 O7 Mo4 166.47(15) . 2_667
O2 Mo3 O7 Mo4 65.85(13) 2_667 2_667
O10 Mo3 O7 Mo4 -92.64(13) . 2_667
O11 Mo3 O7 Mo4 -13.60(11) . 2_667
Mo4 Mo3 O7 Mo4 -56.64(10) . 2_667
O9 Mo3 O7 Mo2 74.8(5) . .
O8 Mo3 O7 Mo2 -77.51(14) . .
O2 Mo3 O7 Mo2 -178.13(12) 2_667 .
O10 Mo3 O7 Mo2 23.38(10) . .
O11 Mo3 O7 Mo2 102.42(12) . .
Mo4 Mo3 O7 Mo2 59.38(8) . .
O9 Mo3 O8 Ag1 -107.2(3) . 1_666
O2 Mo3 O8 Ag1 147.4(3) 2_667 1_666
O10 Mo3 O8 Ag1 -5.7(4) . 1_666
O11 Mo3 O8 Ag1 64.9(6) . 1_666
O7 Mo3 O8 Ag1 65.1(3) . 1_666
Mo4 Mo3 O8 Ag1 -9.2(5) . 1_666
O12 Mo4 O10 Mo3 70.73(17) . .
O13 Mo4 O10 Mo3 178.44(15) . .
O7 Mo4 O10 Mo3 -65.2(3) 2_667 .
O11 Mo4 O10 Mo3 -23.82(13) . .
O11 Mo4 O10 Mo3 -101.11(14) 2_667 .
O12 Mo4 O10 Mo2 -174.13(14) . .
O13 Mo4 O10 Mo2 -66.42(15) . .
O7 Mo4 O10 Mo2 49.9(3) 2_667 .
O11 Mo4 O10 Mo2 91.33(13) . .
O11 Mo4 O10 Mo2 14.03(11) 2_667 .
Mo3 Mo4 O10 Mo2 115.15(19) . .
O9 Mo3 O10 Mo4 -69.54(16) . .
O8 Mo3 O10 Mo4 -175.87(15) . .
O2 Mo3 O10 Mo4 57.1(3) 2_667 .
O11 Mo3 O10 Mo4 22.58(13) . .
O7 Mo3 O10 Mo4 97.80(14) . .
O9 Mo3 O10 Mo2 172.23(12) . .
O8 Mo3 O10 Mo2 65.89(15) . .
O2 Mo3 O10 Mo2 -61.1(2) 2_667 .
O11 Mo3 O10 Mo2 -95.65(12) . .
O7 Mo3 O10 Mo2 -20.44(9) . .
Mo4 Mo3 O10 Mo2 -118.24(19) . .
O6 Mo2 O10 Mo4 168.17(15) . .
O5 Mo2 O10 Mo4 -52.7(4) . .
O4 Mo2 O10 Mo4 64.15(14) . .
O7 Mo2 O10 Mo4 -92.81(14) . .
O11 Mo2 O10 Mo4 -14.54(11) 2_667 .
O6 Mo2 O10 Mo3 -75.05(14) . .
O5 Mo2 O10 Mo3 64.1(4) . .
O4 Mo2 O10 Mo3 -179.07(13) . .
O7 Mo2 O10 Mo3 23.97(11) . .
O11 Mo2 O10 Mo3 102.24(13) 2_667 .
O12 Mo4 O11 Mo3 -80.17(12) . .
O13 Mo4 O11 Mo3 97.5(3) . .
O7 Mo4 O11 Mo3 179.38(12) 2_667 .
O10 Mo4 O11 Mo3 19.32(11) . .
O11 Mo4 O11 Mo3 99.35(11) 2_667 .
O12 Mo4 O11 Mo2 82.17(13) . 2_667
O13 Mo4 O11 Mo2 -100.2(3) . 2_667
O7 Mo4 O11 Mo2 -18.27(11) 2_667 2_667
O10 Mo4 O11 Mo2 -178.33(12) . 2_667
O11 Mo4 O11 Mo2 -98.31(12) 2_667 2_667
Mo3 Mo4 O11 Mo2 162.35(14) . 2_667
O12 Mo4 O11 Mo4 -179.52(12) . 2_667
O13 Mo4 O11 Mo4 -1.9(3) . 2_667
O7 Mo4 O11 Mo4 80.04(12) 2_667 2_667
O10 Mo4 O11 Mo4 -80.02(12) . 2_667
O11 Mo4 O11 Mo4 0.0 2_667 2_667
Mo3 Mo4 O11 Mo4 -99.35(11) . 2_667
O12 Mo4 O11 Mo1 0.9(4) . 2_667
O13 Mo4 O11 Mo1 178.6(4) . 2_667
O7 Mo4 O11 Mo1 -99.5(4) 2_667 2_667
O10 Mo4 O11 Mo1 100.4(4) . 2_667
O11 Mo4 O11 Mo1 -179.6(5) 2_667 2_667
Mo3 Mo4 O11 Mo1 81.1(4) . 2_667
O9 Mo3 O11 Mo4 78.10(13) . .
O8 Mo3 O11 Mo4 -94.3(4) . .
O2 Mo3 O11 Mo4 179.44(13) 2_667 .
O10 Mo3 O11 Mo4 -19.44(11) . .
O7 Mo3 O11 Mo4 -94.48(11) . .
O9 Mo3 O11 Mo2 -23.2(4) . 2_667
O8 Mo3 O11 Mo2 164.4(4) . 2_667
O2 Mo3 O11 Mo2 78.1(4) 2_667 2_667
O10 Mo3 O11 Mo2 -120.8(4) . 2_667
O7 Mo3 O11 Mo2 164.2(5) . 2_667
Mo4 Mo3 O11 Mo2 -101.3(5) . 2_667
O9 Mo3 O11 Mo4 -176.69(12) . 2_667
O8 Mo3 O11 Mo4 10.9(4) . 2_667
O2 Mo3 O11 Mo4 -75.35(12) 2_667 2_667
O10 Mo3 O11 Mo4 85.77(11) . 2_667
O7 Mo3 O11 Mo4 10.73(9) . 2_667
Mo4 Mo3 O11 Mo4 105.21(12) . 2_667
O9 Mo3 O11 Mo1 -85.57(12) . 2_667
O8 Mo3 O11 Mo1 102.0(4) . 2_667
O2 Mo3 O11 Mo1 15.77(10) 2_667 2_667
O10 Mo3 O11 Mo1 176.89(11) . 2_667
O7 Mo3 O11 Mo1 101.85(10) . 2_667
Mo4 Mo3 O11 Mo1 -163.67(13) . 2_667
O12 Mo4 O13 Mo1 -179.88(14) . .
O7 Mo4 O13 Mo1 -75.72(15) 2_667 .
O10 Mo4 O13 Mo1 77.08(16) . .
O11 Mo4 O13 Mo1 2.5(4) . .
O11 Mo4 O13 Mo1 0.72(13) 2_667 .
Mo3 Mo4 O13 Mo1 78.34(19) . .
O3 Mo1 O13 Mo4 3.5(5) . .
O1 Mo1 O13 Mo4 178.10(17) . .
O2 Mo1 O13 Mo4 74.96(16) . .
O4 Mo1 O13 Mo4 -76.75(16) . .
O11 Mo1 O13 Mo4 -0.72(13) 2_667 .
